Carbonitriding is a metallurgical
surface modificationtechnique that is used to increase the surface hardnessof a metal, thereby reducing wear. During the process, atoms of carbon and nitrogen diffuse interstitially into the metal, creating barriers to slip, increasing the hardness and modulus near the surface. Carbonitriding is often applied to inexpensive, easily machined low carbon steel to impart the surface properties of more expensive and difficult to work grades of steel. [ [http://www.key-to-steel.com/Articles/Art126.htm Carbonitriding ] ] Surface hardness of carbonitrided parts ranges from 55 to 62 HRC.
Certain pre-industrial case hardening processes include not only carbon-rich materials such as charcoal, but nitrogen-rich materials such as urine, which implies that traditional surface hardening techniques were a from of carbonitriding.
Carbonitriding is similar to
gascarburization with the addition of ammoniato the carburizing atmosphere. which provides a source of nitrogen. Nitrogenis adsorbed at the surface and diffuses into the workpiece along with carbon. Carbonitriding (around 850 °C / 1550 °F) is carried out at temperatures substantially higher than plain nitriding (around 530 °C / 990 °F) but slightly lower than those used for carburizing (around 950 °C / 1700 °F) and for shorter times. Carbonitriding tends to be more economical than carburizing, and also reduces distortion during quenching. The lower temperature allows oil quenching, or even gas quenching with a protective atmosphere.
Characteristics of carbonitrided parts
Carbonitriding forms a hard, wear resistant case, typically .07mm -.5mm thick, and generally has higher
hardenessthan a carburized case. Case depth is tailored to the application, and a thicker case, increases wear life of the part. Carbonitriding alters only the top layers of the workpiece; and does not deposit an additional layer, so the process it does not significantly alter the dimensions of the part.
Maximum case depth is typically restricted to 0.75mm; case depths greater than this take too long to diffuse to be economical. Shorter processing times are preferred to restrict the concentration of nitrogen in the case, as nitrogen addition is more difficult to control than carbon. An excess of nitrogen in the work piece can cause high levels of
retained austeniteand porosity, which are undesirable in producing a part of high hardness.
Carbonitriding also has other advantages over carburizing; it has a greater resistance to softening during
temperingand increased fatigue and impact strength. It is possible to use both carbonitriding and carburizing together to form optimum conditions of deeper case depths and therefore performance of the part in industry. This method is applied particularly to steels with low case hardenability, such as the seat of the valve. The process applied is initially carburizing to the required case depth (up to 2.5mm) at around 900-955°C, and then carbonitriding to achieve required carbonitrided case depth. The parts are then oil quenched, and the resulting part has a harder case than possibly achieved for carburization, and the addition of the carbonitrided layer increases the residual compressive stresses in the case such that the contact fatigue resistance and strength gradient are both increased.
Typical applications for case hardening are
gear teeth, cams, shafts, bearings, fasteners, pins, automotive clutch plates, tools, and dies.
last = Kalpakjian
first = Serope
authorlink = Serope Kalpakjian
coauthors = Steven Schmid
title = Manufacturing, Engineering & Technology
publisher = Prentice Hall; 5 edition
date = 2005
location = New York
pages = 137-138
isbn = 0131489658
Wikimedia Foundation. 2010.
Look at other dictionaries:
Carbonitriding — Carbonitriding. См. Нитроцементация. (Источник: «Металлы и сплавы. Справочник.» Под редакцией Ю.П. Солнцева; НПО Профессионал , НПО Мир и семья ; Санкт Петербург, 2003 г.) … Словарь металлургических терминов
carbonitriding — Смотри Карбонитрирование … Энциклопедический словарь по металлургии
Нитроцементация — Carbonitriding Нитроцементация. Процесс создания упрочненного слоя, при котором подходящая сталь нагревается выше нижней температуры превращения в газообразной атмосфере химического состава, способного вызвать одновременную диффузию углерода и… … Словарь металлургических терминов
Карбонитрирование — [carbonitriding] ХТО, заключающийся в комбинированном диффузном насыщении поверхностного слоя металла (изделия) N и С, приводящем к образованию слоя, содержащего карбиды, нитриды или карбо нитриды, ниже которого находится обогащенный азотом… … Энциклопедический словарь по металлургии
Tenifer — is a trademarked name for the end result of a chemical bath nitriding process that embeds nitrogen into an iron containing alloy to create a corrosion resistant finish that is a dull grey in color and extremely hard. The generic term for this… … Wikipedia
Case hardening — or surface hardening is the process of hardening the surface of a metal, often a low carbon steel, by infusing elements into the material s surface, forming a thin layer of a harder alloy. Case hardening is usually done after the part in question … Wikipedia
Heat treatment — is a method used to alter the physical, and sometimes chemical, properties of a material. The most common application is metallurgical. Heat treatments are also used in the manufacture of many other materials, such as glass. Heat treatment… … Wikipedia
Parkerizing — (also called phosphating and phosphatizing) is a method of protecting a steel surface from corrosion and increasing its resistance to wear through the application of an electrochemical phosphate conversion coating. Parkerizing is usually… … Wikipedia
Carburization — (often referred to as carburizing) is a heat treatment process which iron or steel is heated to below the melting point in the presence of a solid, liquid, or gaseous material which decomposes so as to liberate carbon when heated to the… … Wikipedia
Nitridization — Nitridization, also known as nitriding, is a process which introduces nitrogen in the surface of a material. It is used in metallurgy, for example, for case hardening treatment of the steel surface.Nitriding is widely used in automotive,… … Wikipedia